Research Article  Open Access
Jiaqi Yu, Yi Li, Fei Teng, Jicai Liang, Xiangfeng Lin, Ce Liang, Guangyi Chen, Guangping Sun, "Research on the Cross Section Forming Quality of ThreeDimensional Multipoint Stretch Forming Parts", Advances in Materials Science and Engineering, vol. 2018, Article ID 4265617, 11 pages, 2018. https://doi.org/10.1155/2018/4265617
Research on the Cross Section Forming Quality of ThreeDimensional Multipoint Stretch Forming Parts
Abstract
This paper introduced the basic principle and main influencing factors of the threedimensional multipoint stretch forming process and investigated the optimized scheme of the cross section forming quality. The main factors affecting the stretch forming process were studied by the orthogonal test through the numerical simulation technique. In the case of a good target shape, the best combination of forming parameters was established by using the range method. The crosssectional distortion of the formed profile is the smallest when the prestretching amount is 1% of the profile length, the poststretching amount is 0.8% of the profile length, the number of the die heads is 12, and the friction coefficient is 0.15. The optimal combination of forming parameters was verified by the multipoint bending test.
1. Introduction
Stretch forming is a method of bending parts under a combination of stretching and bending moments. The most challenging problem in the automobile industry now is to reduce the consumption of gasoline. Therefore, lightweight structure design is attracting much attention, and the aluminum alloy is widely used due to its strong stiffness and lightweight [1]. Threedimensional multipoint stretch forming is a rapid flexible forming technique which is different from the traditional bending forming. Its flexible bending head makes the bending radius change, so it can be widely applied to many profiles [2, 3]. In addition to the common problems such as wrinkle, springback, and fracture in sheet forming, there are some special problems in the forming parts, such as crosssectional distortion. The common problem of thinwalled section stretch forming is the crosssectional distortion, and the main defects are collapse and bulging [4–8].
In order to achieve the skeleton of the spatial structure with complex threedimensional surface, many scholars had done some researches. By using the numerical simulation technology, Paulsen and Welo made an arrangement for the degree of factors affecting the distortion on the cross section [9]. Miller et al. did a detailed research on the influence of stretchbending process parameters on formability, then optimized the parameters, and got the conclusion that the tension force can reduce springback [10]. Paulsen and Welo discussed the collapse of the cross section and obtained a fairly complex equation set [11]. Chunguo et al. systematically studied the basic theory and technology of sheet metal multipoint forming process and named the adjustable forming method “multipoint forming” for the first time [12]. A finite element simulation trajectory design method based on deformation control was proposed by Li et al. [13]. For different loading methods of two different aluminum profiles, Clausen et al. used the experimental method and the finite element analysis, and they found that the crosssectional geometry and prestretching affect the distortion greatly [14]. Diao et al. came up with the mechanical property parameters of materials through the relevant mechanical experiments of rectangular aluminum alloy profiles [15].
In this paper, under the precondition that the target shape was well bent, the numerical simulation technology was used to simulate the stretch forming process according to the characteristics that the section of rectangular thinwalled hollow aluminum alloy is easy to deform. During the stretch forming process, the main process parameters influencing the crosssectional distortion were studied by the orthogonal test; then, the effect of a single factor was discussed; and finally, the optimal combination of process parameters by the range method was determined.
2. ThreeDimensional Multipoint Stretch Forming Process
2.1. Basic Principle
Multipoint forming (MPD) is an advanced forming technique which is based on the principle of flexible multipoints forming technology. The traditional monolithic die is discretized to form a flexible die with a variable shape and adjustable height. It can be adjusted in horizontal and vertical directions to achieve threedimensional stretch bending [16]. Compared with the traditional die, the unit body of threedimensional stretched die has the advantages of wide processing profile length, simple shape adjustment, and application of various types of cross sections. The reconfigurable die with multiple units are used to reconstruct the die surface by changing the space position during the flexible stretch forming process, as shown in Figure 1 [17, 18].
(a)
(b)
The flexible stretch forming machine is made of the proper installation of several die heads on the worktable of the bending machine combining with the traditional stretch forming method, and the structure is shown in Figure 2.
(a)
(b)
2.2. Main Factors Affecting the Multipoint Stretch Forming
The profile stretching is usually stretched to the plastic state and is fitted on the contact surface of the bending die to get the final shape. The most important crosssectional distortions during bending are collapse and bulging, so it is necessary to find a practical solution.
The main forming process of threedimensional stretch forming is divided into three steps: prestretching process, bending process, and poststretching process, that is, the PMP method. First, the clamps are controlled along the displacement direction of the profile for the poststretching process. The amount of prestretching should make the plastic deformation of the profile appropriate because too much prestretching will lead to section collapse and fracture of the profile. Second, the clamps drive the profile to fit the dies. The bending process includes two stages: bending in horizontal and bending in vertical. The profile is bent in the horizontal plane first and is bent along the zaxis then. Last, the poststretching is done for the curved profile to improve the forming precision. The reference point of the clamp controls the profile to move in the direction of the part. In the whole process of bending, the size of the friction coefficient and the number of multipoint die heads also affect the quality of forming parts. The PMP process flow diagram is shown in Figure 3.
3. Numerical Simulation
The finite element analysis method can simplify the profile reasonably. The finite element model can be used to study the stress and strain distribution, springback, wrinkling, rupture, collapse, bulging, and other problems during the forming process. By changing the process parameters, the influence of the parameters on the forming quality was studied, so that the adjustment can be made properly to get the optimal solution into actual experimental production. In this paper, the threedimensional multipoint stretch forming process of the aluminum alloy rectangular profile was numerically simulated by using the finite element analysis software ABAQUS. The section size is shown in Figure 4 (unit: mm). This paper used the aluminum alloy AA6082 as the experiment profile, its stressstrain curve is shown in Figure 5, and the material parameter is shown in Table 1. The length of the profile is 3200 mm. The target bending radius is 2500 mm, and both the horizontal bending angle and the vertical bending angle are 30°. The experiment is mainly to form the whole profile by stretch forming.
 
Note: E represents the modulus of elasticity, represents the Poisson ratio, σ_{0} represents the yield stress, σ_{b} represents the tensile strength, and ρ represents the density. 
3.1. Reasonable Simplification of Flexible ThreeDimensional Stretch Forming
The flexible threedimensional stretch forming process of the profile is a complex nonlinear springback forming problem, which includes the nonlinearity of materials and the nonlinearity of boundary conditions and so on. A too complicated model not only prolongs the calculation time but also leads to the inaccuracy of the calculation results. In order to get accurate simulation, the finite element model of flexible threedimensional stretch forming was reasonably simplified.
3.1.1. Simplification of Stretch Forming Process
In the finite element analysis of flexible stretch forming, it is important to simulate the profile gradually fitting the flexible dies under the action of the linear displacement of the clamps. The unnecessary components of the bending machine were simplified; that is, to say, the forming process of stretch bending can only be driven by the clamp to fit the die body.
3.1.2. Simplification of Operation Process
Half of the profile was selected for simulation in consideration of the symmetry of the profile and operation, and it was also convenient to observe the distortion of the cross section and save time. Because of the symmetry of the profile and the operation, in the finite element analysis of the threedimensional multipoint flexible stretch forming, half of the dies, clamps, and profile which were selected to simulate can facilitate the observation of crosssectional distortion and shorten the calculation time. Therefore, the finite element model presented in this paper is composed of onehalf of each component.
3.1.3. Simplification of Shape
Since the profile has the regular rectangular section, in the finite element model, the shape and the size of the aluminum profile were designed in 1 : 1 scale according to the actual size, and the threedimensional solid element was selected. The shape of the die that controls the horizontal bending on the bending machine is shown in Figure 7. The limit screw that controls vertical bending on the bending machine was defined in the same shape as the die unit in the model and was simplified as a discrete rigid body. The clamps used the same shape of rectangular threedimensional shell structure as the profile, with a length of 50 mm. Figure 6 is the assembly sketch of the profile, and Figure 7 is the parts diagram. The target shape of the aluminum profile is shown in Figure 8.
(a)
(b)
(c)
(d)
3.1.4. Reasonable Mesh Partitioning
Because the profiles, clamps, and multipoint die heads in this paper are all regular shapes, this paper adopted structured grid technology. The aluminum profile unit used a hexahedron structure, and the wall thickness was divided into a layer of mesh; that is, the mesh size was 2 × 2 mm, and the mesh size in length and width direction was 2.5 × 2.5 mm. Since the horizontal multipoint die, vertical multipoint die, and clamp have a relatively small influence on the calculation results and are not the main part of the study, the mesh size was designed to be 5 × 5 mm to save calculation time, such as Figure 7.
The finite element model was divided into three submodels and five analytic steps, which were defined as the horizontal bending model, vertical bending model, and poststretching model, respectively. The horizontal bending model included the initial analysis step, the prestretching process, and the horizontal bending stage. The vertical bending model included the vertical bending stage. And the poststretching model included the poststretching process. After completing each model task successfully, it was used as a predefined field to start the next model run.
3.2. The Orthogonal Test
The orthogonal test is a design method which is based on the orthogonality of the data to design the scheme. It has the advantage of being able to obtain reliable and representative test results in test times as few as possible. Through the analysis and integration of the test results, the best test conditions are selected as the optimal level combination of each factor. The orthogonal test is beneficial to improve production efficiency, shorten working time, and improve process quality, so it is widely used in the field of automobile manufacture and aerospace to deal with multifactor problems.
Proper prestretching and poststretching will affect the distortion of the cross section and then change the precision of the forming part. The number of die heads also affects the wrinkling and deformation of the profile during the bending process. Therefore, this paper focused on the experimental factors including prestretching, poststretching, the number of die heads, and the friction coefficient, defining A as the amount of prestretching, B as the amount of poststretching, C as the number of die heads, and D as the amount of friction coefficient. The assessment index was the crosssectional distortion of the stretch forming parts, and the collapse rate and the bulging rate were taken as the evaluation criteria. Four experimental factors were selected. Therefore, the orthogonal test was designed with four factors and four levels. Altogether, 16 groups of experiments were carried out, which is shown in Table 2.

3.3. Assessment Index
The method of quantitative analysis was used to deal with the distortion of the cross section. Select the maximum level of various factors as a parametric combination for the boundary simulation. The combination was C = 12, A = B = 1.4% L, and D = 0.2. Figure 9 is the numerical simulation of the profile deformation. To facilitate observation, the distortion diagram of the cross section is plotted as shown in Figure 10. What this paper mainly measured was how the section changes after the horizontal bending, the vertical bending, and the poststretching. Measure the outermost midpoint change in the symmetry section. The gap amount (ΔB and ΔH) was used to describe the amount of profile crosssectional distortion. Among them, the collapse rate δ = ΔH/H, and the bulging rate η = ΔB/B.
4. Results and Analysis
4.1. Orthogonal Test Result
The orthogonal test method not only makes the plan have some advantages but also reduces the test points, so that a small number of experiments can get rich information, control the test interference effectively, and get a comprehensive conclusion [19]. The range method is an analysis method which is easy to grasp and has less calculation. It is used to screen the initial test, to seek the optimal production condition and the process and so on. The crosssectional distortion of the horizontal bending process, the vertical bending process, and the poststretching process was measured. And the average number of arithmetical number corresponding to the level number was recorded as ki (i = 1, 2, 3, 4). The difference between the max {ki} and the min {ki} on any column was the extreme R. Data record analyses in Table 3 are obtained by the range method.
 
Note: δ_{h} represents the collapse rate in the horizontal stage, δ_{v} represents the collapse rate in the vertical stage, δ_{p} represents the collapse rate in the poststretching process, η_{h} represents the bulging rate in the horizontal stage, η_{v} represents the bulging rate in the vertical stage, and η_{p} represents the bulging rate in the poststretching process. 
4.2. Influence of Single Factor on CrossSectional Distortion of Each Process
The following graphs are the corresponding trend maps at different levels of influence factors. This paper discussed the crosssectional variation trend in bending in the horizontal, vertical, and poststretching process (defining bending in the horizontal stage, bending in the vertical stage, and poststretching process as two processes or three stages). The horizontal coordinate is the level, and the longitudinal coordinate is a cross section variable obtained by the use of the range method.
4.2.1. Influence of Prestretching
Figure 11 is a trend diagram of the variation of the crosssectional distortion with the amount of prestretching during the stretch forming. As can be seen from Figure 11, during the bending process, when the prestretching A = 1.0% L (Figure 11(a)), δ is the smallest, and the tendency of bending in the horizontal stage, bending in the vertical stage, and the poststretching process is almost the same. They both reduce, then increase, and finally decrease. When the prestretching A = 1.2% L (Figure 11(a)), δ is the biggest. η is the smallest when A = 1.2% L (Figure 11(b)). At the same time, the effect of prestretching on the rate of bulging does not have a large amount on collapse.
(a)
(b)
4.2.2. Influence of Poststretching
The changing trend of crosssectional distortion with the amount of poststretching during the stretch forming process is shown in Figure 12. As can be seen from Figure 12(a), δ increases when B increases from 0.8% L to 1.2% L during the both three stages. When B increases to 1.4% L, δ decreases in the vertical bending stage and poststretching process. δ becomes larger in the horizontal bending stage. The reason is that the amount of poststretching was applied to the poststretching process and that it had a great influence on the distortion. δ is the smallest when B = 0.8% L during the two processes. It can be seen from Figure 12(b) that the influence of the poststretching on the bulging rate is not obvious in the horizontal direction. The others have obvious fluctuations. In the vertical bending stage, bulging η reduces and then increases gradually. As for the poststretching process, it is a bit different from the bending in the vertical stage, and when B > 1.2% L, η decreases slightly. But η is the smallest when B = 1.0% L during the two processes.
(a)
(b)
4.2.3. Influence of the Number of Die Heads
The changing trend of crosssectional distortion with the number of die heads during the stretch forming process is shown in Figure 13. As can be seen from Figure 13(a), the collapse rate δ decreases with the increase of C in both horizontal and vertical stages, which can reflect the advantage of multipoint flexible forming. And the number of die heads can reduce the collapse effectively. As shown in Figure 13(b), the vertical bending and the poststretching process tend to have similar effects on the bulging rate η, but the horizontal bending is different from them. In general, the distortion of the cross section is the largest when C = 6 and the distortion of the cross section is the smallest when C = 12. Figure 14 is the assembly drawing with different number of die heads.
(a)
(b)
(a)
(b)
(c)
(d)
4.2.4. The Influence of Friction Coefficient
Figure 15 is the influencing trend of the friction coefficient on the crosssectional distortion during the stretch forming process. From Figure 15(a), when D = 0.15, δ is the smallest in the both two process. During the bending process, the crosssectional distortion has a upward trend, then decreases, and finally increases. From Figure 15(b), as for the effect of friction coefficient on the horizontal stage, when the friction between 0.12 and 0.15 increases, the bulging rate becomes smaller. The tendency of bending in the vertical stage and the poststretching process are almost the same. They both increased, then reduced, and finally decreased. Generally speaking, when D = 0.15, the overall distortion of the cross section is minimal.
(a)
(b)
4.3. Process Parameters Optimization and Verification Experiment
The analysis from 4.2 is based on the size of the collapse rate and the bulging rate; therefore, the smaller the amount, and the better the result. The best combination of process parameters is C4D3, where C = 12 and D = 0.15. Further analyses are needed for the selection of prestretching and poststretching. Comparing ki of the factors A and B in Table 3 (the smaller ki indicates the smaller degree of influence on behalf of this level) and the combination of the prestretching and poststretching are designed in Table 4.

From Table 4, it can be seen that the best combination of the bending process for reducing the collapse rate is A2B1, and the best combination of the stretch forming process for reducing bulging is A3B2. The comparison of several groups of data shows that not all the indicators are consistent, but the general trend is the same. In order to find the optimal combination, the following two sets of process parameters are numerically simulated to determine the optimal combination, and the experimental verification is carried out in the stretch forming test.
According to the combination of the two sets of parameters obtained from the simulation, the forming test is arranged to verify the simulation results and the optimal combination of parameters is discussed (the profilerelated parameters used in the stretchbending forming test are consistent with the simulation parameters). Figure 16 is a multipoint stretch forming test. Figure 18 shows the crosssectional distortion of the two process parameters.
As can be seen from the stress clouds of the simulation in Figure 17, on the one hand, the stress distribution at section A2B1C4D3 is mainly green, while that at section A3B2C4D3 is yellow as a whole. From the distribution of stress cloud, the yellow part of the stress value is greater than the green part of the stress value; therefore, the overall stress distribution of A2B1C4D3 is smaller than that of A3B2C4D3. On the other hand, the crosssectional distortion of A2B1C4D3 is smaller than A3B2C4D3. So the optimal combination of the finite element simulation results is A2B1C4D3. As shown in Figure 18, the crosssectional distortion of A2B1C4D3 is smaller than that of A3B2C4D3 in each process step of the forming test, so the best combination is A2B1C4D3 which is in agreement with the results obtained from the numerical simulation.
(a)
(b)
5. Conclusion
This paper studied the threedimensional multipoint stretch forming of the aluminum alloy rectangular profile and used the finite element analysis method to investigate the influence of prestretching, poststretching, the number of die heads, and the coefficient of friction on the distortion of the cross section. The optimal combination of process parameters was determined and was verified by the forming test.(1)The effect of collapse on the profile is greater than bulging. The collapse rate decreases with the increase of the prestreching amount from 0.8% L to 1.0% L. As the prestretching amount continues to increase, the crosssectional distortion becomes larger and then decreases slightly. When prestretching amount is 1.2% L, the collapse rate is the smallest.(2)After unloading, the profile enters the stage of the poststretching process. When the amount of the poststretching amount is increased from 0.8% L to 1.2% L, the collapse rate increases generally. Therefore, the larger the poststretching amount, the larger the collapse rate. However, there are little fluctuations during the horizontal bending process on the bulging problem.(3)The number of die heads has great influence on the accuracy of profile forming. When the number of die heads increase from 6 to 12, the collapse obviously decreases and the crosssectional distortion is obviously improved.(4)When the friction coefficient increases from 0.01 to 0.2, the crosssectional distortion in the horizontal direction is not large, but when it reaches 0.15, the overall crosssectional distortion becomes small.(5)By taking the orthogonal test and forming test on rectangular hollow section profile, the optimal combination of threedimensional multipoint stretch forming is as follows: the prestretching amount is 1.0% L, the poststretching amount is 0.8% L, the number of die heads is 12, and the friction coefficient is 0.15.
Conflicts of Interest
The authors declare that they have no conflicts of interest.
References
 M. Geiger and A. Sprenger, “Controlled bending of aluminum extrusions,” CIRP Annals, vol. 47, no. 1, pp. 197–202, 1998. View at: Publisher Site  Google Scholar
 L. Jicai, T. Fei, G. Song et al., “Key technologies research on the iterative dieface adjustment in the forming process of flexible threedimensional stretchbending,” Journal of Mechanical Engineering, vol. 49, no. 17, pp. 187–192, 2013. View at: Publisher Site  Google Scholar
 G. Song, L. Jicai, C. Guangyi et al., “Rapid adjusting of fundamental units in process of flexible 3D stretchbending,” Journal of Jilin University: Engineering and Technology Edition, vol. 44, no. 6, pp. 1723–1728, 2014. View at: Google Scholar
 L. Zhiwei, L. Mingzhe, and H. Qigang, “Multipoint forming with wrinkle resistance function and its forming accuracy,” Journal of Mechanical Engineering, vol. 48, no. 12, pp. 56–62, 2012. View at: Publisher Site  Google Scholar
 G. Zhengwei, C. Zhongyi, and X. Hong, “Numerical analysis and optimization of stretchbending process,” Journal of Jilin University: Engineering and Technology Edition, vol. 39, no. 5, pp. 1167–1171, 2009. View at: Google Scholar
 Z.Y. Cai, S.H. Wang, X.D. Xu, and M.Z. Li, “Numerical simulation for the multipoint stretch forming process of sheet metal,” Journal of Materials Processing Technology, vol. 209, no. 1, pp. 396–407, 2009. View at: Publisher Site  Google Scholar
 L. G. Brazier, “On the flexure of thin cylindrical shells and other “thin” sections,” Proceedings of the Royal Society of London, vol. 116, no. 773, pp. 104–114, 1927. View at: Publisher Site  Google Scholar
 X.L. Zhang, X.X. Li, X.B. Zhou, and M. Jin, “Finite element simulation for stretchwrap bending of aluminum profile with complex cross section,” Journal of Plasticity Engineering, vol. 11, no. 4, pp. 44–47, 2004. View at: Google Scholar
 F. Paulsen and T. Welo, “Application of numerical simulation in the bending of aluminumalloy profiles,” Journal of Materials Processing Technology, vol. 58, no. 23, pp. 274–285, 1996. View at: Publisher Site  Google Scholar
 J. E. Miller, S. Kyriakides, and A. H. Bastard, “On bendstretch forming of aluminum extruded tubes I experiments,” International Journal of Mechanical Sciences, vol. 43, no. 5, pp. 1283–1317, 2001. View at: Publisher Site  Google Scholar
 F. Paulsen and T. Welo, “Crosssectional deformations of rectangular hollow sections in bending: part II analytical models,” International Journal of Mechanical Sciences, vol. 43, no. 1, pp. 131–152, 2001. View at: Publisher Site  Google Scholar
 L. Chunguo, L. Mingzhe, C. Zhongyi, and C. Qingmin, “Research on multipoint closedloop forming of 3D sheet metal parts,” China Mechanical Engineering, vol. 11, no. 12, pp. 1326–1329, 2000. View at: Google Scholar
 X. Li, X. Zhou, C. Jin, and C. Hao, “Design of stretch bending trajectory based on finite element simulation for threedimensional profile parts,” Acta Aeronautica et Astronautica Sinica, vol. 30, no. 3, pp. 544–550, 2009. View at: Google Scholar
 A. H. Clausen, O. S. Hopperstad, and M. Langseth, “Stretch bending of aluminum extrusions for car bumpers,” Journal of Materials Processing Technology, vol. 102, no. 1, pp. 241–248, 2000. View at: Google Scholar
 K. Diao, X. Zhou, X. Li, and B. Criqui, “An investigation of material properties of aluminum extrusion 6082(T5) and the establishment of FLD,” China Mechanical Engineering, vol. 15, no. 13, pp. 1202–1204, 2004. View at: Google Scholar
 L. Yi, L. Jicai, T. Fei, L. Ce, and Y. Jiaqi, “Multiphase iterative compensation method of die shape optimization for multipoint stretch bending profile,” Journal of Jilin University: Engineering and Technology Edition, vol. 46, no. 6, pp. 1961–1966, 2016. View at: Google Scholar
 J.C. Liang, S. Gao, F. Teng, and X.J. Song, “Flexible 3D stretchbending technology for aluminum profile,” International Journal of Advanced Manufacturing Technology, vol. 71, no. 9–12, pp. 1939–1947, 2014. View at: Google Scholar
 X. P. Gong, M. Z. Li, Z. Q. Hu, and Z. Y. Cai, “Research on continuous multipoint forming technology for threedimensional sheet metal,” International Journal of Materials and Product Technology, vol. 38, no. 23, pp. 210–222, 2010. View at: Publisher Site  Google Scholar
 L. Jicai, S. Mei, L. Yi et al., “Influence factor analysis of gas fingering defect in gasassisted injection dieing of automobile handle,” Journal of Mechanical Engineering, vol. 44, no. 12, pp. 303–313, 2008. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2018 Jiaqi Yu et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.